499

Tribology Letters, Vol. 18, No. 4, April 2005 ( 2005) DOI: 10.1007/s11249-005-3610-0

Friction coefﬁcient of soft contact lenses: measurements and modeling A.C. Rennie, P.L. Dickrell and W.G. Sawyer* Department of Mechanical and Aerospace Engineering, University of Florida, Gainesville, FL 32611, USA

Received 12 October 2004; accepted 16 January 2005

Tribological conditions for contact lenses have very low contact pressures in the range 3–5 kPa and sliding speeds around 12 cm/s. Using a microtribometer a series of experiments was run on commercially available contact lenses made from Etaﬁlcon-A. These tests were run using 10–50 mN of normal load at speeds from 63 to 6280 lm/s using a 1-mm radius glass sphere as a pin. The resulting contact pressures are believed to be nearly an order of magnitude larger than the targeted 3–5 kPa. It is hypothesized that the viscoelastic nature of the hydrogel, viscous shearing of the packaging solution, and interfacial shear between the glass sphere and the contact lens all contribute to the friction forces. A model that includes all three of these contributors is developed and compared to the experimental data. The experimental friction coeﬃcients vary from l = 0.025 to 0.075. The calculated ﬂuid ﬁlm thicknesses were between 1 and 30 nm. The average surface roughness of the lens and the glass sphere are Ra=15 nm and Ra=8 nm, respectively, suggesting that the contact is not in full elastohydrodynamic lubrication. Finally, the largest contributors to the friction force in these experiments were found to be viscous dissipation within the hydrogel and interfacial shear within the contact zone. KEY WORDS: contact lens, hydrogel friction, microtribology, microtribometer

1. Introduction Hydrogels are polymer matrices that contain 30–70% water [1] and are the primary material for soft contact lenses. Although soft materials are well suited for the eye, a signiﬁcant fraction of people are unable to wear contact lenses because of extensive eye irritation. There is an existing clinical hypothesis that ocular comfort is related to friction. The mechanical properties of hydrogels are extremely sensitive to water content and humidity, and contact pressure is known to cause redistribution and/or reduction of the water content of hydrogel materials [2]. Therefore, tribological testing of hydrogels must be done under low contact pressure conditions. Nairn and Jiang [3] reported the friction coeﬃcients of polyhydroxy ethyl methacrylate (p-HEMA) based lenses to be in the range of l = 0.060–0.115 using a custom-built pin-on-disk tribometer. The contact pressure in their study was 3.5 kPa. Freeman et al. [4] reported the friction coeﬃcient of ﬂat disks of p-HEMA hydrogels to be in the range of l = 0.02–1.7 over a wide range of applied load, lubrication, hydrogel crosslink density, and degree of hydrogel hydration again using a special purpose tribometer. This study aims to identify the various contributions to friction force in a microtribological contact with a saturated hydrogel. The in vitro conditions are selected *To whom correspondence should be addressed. E-mail: [email protected]ﬂ.edu

to come as close as possible to the pressures and speeds experienced in vivo using existing microtribometry. Blinking is assumed to be the primary force and motion contribution for contact lens tribology. Estimates of the contact pressure created by the eyelid during blinking range from 3.5 to 4.0 kPa and blinking speed average around 12 cm/s [3,5,6]. This combination of low contact pressure and moderate sliding speed are challenging. In this study a reciprocating microtribometer is used to explore the contact pressure and speed dependence of friction coeﬃcient measurements of contact lenses.

2. Experimental setup Tribology experiments were run on a reciprocating microtribometer that uses dual glass ﬂexures to apply mN-range normal loads and react mN-range frictional forces [7]. The tribometer is mounted on an active vibration isolation granite table inside a softwall cleanroom. The apparatus is shown in ﬁgure 1. For these experiments commercially available soft contact lenses made from Etaﬁlcon-A [8] were mounted onto plastic base curves that match the internal radius of curvature of the lenses. The pin sample is a borosilicate crown glass sphere of radius 1mm, and the base curves and contact lenses have a radius of curvature of approximately 7.1 mm. Material properties and surface characterization of the samples are given in table 1. All tests were run using the same experimental procedure: (1) a clean and dry base curve is positioned on 1023-8883/05/0400–0499/0 2005 Springer Science+Business Media, Inc.

500

A.C. Rennie et al./Friction coeﬃcient of soft contact lenses Table 2. Experimental conditions. Applied normal load Reciprocating amplitude Reciprocating frequency Sliding speed Relative humidity Sampling rate

Figure 1. Photograph of the micro-tribometer setup showing: (1) glass ﬂexure to react normal load and friction forces, (2) optical sensor for vertical deﬂections, (3) mirrors, (4) optical sensor for horizontal deﬂections, (5) borosilicate crown glass pin with a 7 mm radius of curvature (a) 1-mm radius sphere was used in this study), (6) EtaﬁlconA contact lens, (7) reciprocating stage, (8) LVDT for stage position measurements, and (9) plastic base curve used to hold the contact lens. Table 1. Material properties of the glass sphere and the Etaﬁlcon-A contact lenses. Glass sphere Average roughness Radius of curvature Elastic modulus Poisson ratio Thickness a

Ra R E m c

a

8 nm 1 mmb 60 GPab 0.30

Contact lens 15 nm[12] 7.1 mmb 255 kPab 0.45b 100 lmb

Collected using a scanning white-light interferometer. Manufacturer reported values.

b

the microtribometer reciprocating stage, (2) a clean and dry glass sphere is mounted to the glass cantilever, (3) a new contact lens package is opened, (4) the lens is removed from the package by hand (only the back side

Fn

V

3–20 mN 0.60 mm 0.07–6.66 Hz 63–6280 lm/s 46–51% 100 Hz

of the lens is handled), (5) the lens is transferred onto the base curve, (6) ﬁnal positioning of the lens on the base curve is done with clean stainless steel tweezers, (7) the lens and base curve assembly is positioned under the borosilicate pin near the apex of the curve, (8) a normal load is applied, and (9) the test is initiated and run for a prescribed number of cycles (based on sliding speed). Steps 3–8 are completed in less than 1 min or the test is abandoned. The experimental conditions used in this study are given in table 2.

3. Modeling The modeling of the experiments done on these contact lenses begins by assuming that the lens can be reasonably modeled with a modiﬁed Winkler surface [9]. The modiﬁcation is the inclusion of a viscous damper into the traditional bed-of-springs elements. This is given by equation (1) where P (Pa) is the contact pressure, E (Pa) is the elastic modulus, m is Poisson’s ratio, c (mm) is the thickness, d (mm) is the normal deformation, b ((Pa s)/mm) is the viscous coeﬃcient, and d_ (mm/s) is the rate of normal deformation. A contact schematic is shown in ﬁgure 2. P¼

E d þ bd_ ¼ ks d þ bd_ ð1 v2 Þc

ð1Þ

The normal load Fn for quasi-static indentation of two spheres can be found by integrating equation (1) over

–

–

–

Figure 2. A contact schematic and nomenclature showing the modiﬁed Winkler foundation material model. The meniscus, lens thickness, ﬂuid ﬁlm thickness, surface roughness, and deformation are all exaggerated.

501

A.C. Rennie et al./Friction coefﬁcient of soft contact lenses

the circular contact of diameter 2b in polar coordinates, where r is the radial coordinate going from 0 to b, and h is the angular coordinate with h=0 lying along the direction of travel. Fn ¼

Z2p Zb 0

P rdr dh ¼ ks

0

Z2p Zb 0

d rdr dh ﬃ ks

pb4 4R0

ð2Þ

0

In equation (2), R¢ is the composite radius of curvature as given by equation (3), where R1 and R2 are the radii of curvature of the two spheres. The approach of centers d for this contact is given by equation (4). The relationship between d and Fn requires solving equation (2) for the contact radius and inserting this result into equation (4). 1 1 1 ¼ þ 0 R R1 R2 d ¼ R1 þ R2

qﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ qﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ R21 b2 R22 b2

ð3Þ

ð4Þ

For the Hertzian contact problem the approach of centers is given by equation (5) [10], where the eﬀective elastic modulus E¢ is given by equation (6) (the borosilicate glass sphere is assumed to be rigid with respect to the contact lens material). 1=3 1 9 F2n d¼ ð5Þ 2 2 E02 R0 E0 ﬃ

E 1 m2

A plot of the normal load versus ﬁlm penetration is shown in ﬁgure 3, and curve ﬁts of equations (4) and (5) are shown on the plot. From these curve ﬁts an elastic modulus E for the foundation model (equation (1)) and a Hertzian contact model (equation (5)) are selected (for both models m=0.45 is used in the curve ﬁtting). It is

noteworthy that the elastic modulus for the foundation model was found to be 260 kPa and the manufacturer reported modulus is 255 kPa. In ﬁgure 2, a schematic for a sphere sliding across the modiﬁed elastic foundation with viscous damping is shown. The deformation d under the sphere of radius R is given in polar coordinates by equation (7). The rate of change of the deformation under the sphere is given by equation (8), where V is the sliding speed. pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ d ¼ d R þ R2 r2 ð7Þ r cosðhÞV d_ ¼ pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ R2 r2

ð8Þ

Combining equations (4), (7) and (8) gives a compact expression for the pressure distribution under a moving sphere, which is given by equation (9). Because of the (h) term in the viscous damping portion of the foundation model, the contribution of this additional term to the integrated pressure distribution is zero (i.e. the contact area remains constant for any sliding speed and thus equation (2) holds for all sliding speeds that do not create negative pressures under the contact). hpﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃi r cosðhÞV 2 2 2 2 Pr;h ¼ R r R b ks þ pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ b ð9Þ R2 r2 Using the substitution r ¼ R sinð/Þ the pressure distribution acting normal to the glass sphere is given by equation (10). The contact zone is over the range of angular coordinate / from / ¼ 0 to /max, which is given in equation (11). P/;h ¼ ½Rðcosð/Þ cosð/max ÞÞks þ ½cosðhÞ tanð/ÞVb ð10Þ /max ¼ sin1

b R

ð11Þ

The diﬀerential friction force, dfve, is the projection of the normal pressure on the sphere opposing the direction of motion multiplied by the diﬀerential area, which is given in equation (12). dfve ¼ P/;h sinð/Þ cosðhÞ dA

ð12Þ

The asymmetric pressure distribution (equation (10)) of the viscoelastic foundation model results in a net friction force fve for this contact geometry. The integral for the viscoelastic contribution to friction force is given by equation (13), and the solution to this integral is given by equation (14), where the dimensionless normal load Fn* is given by equation (15). Figure 3. Experimental data collected by performing an indentation test with the microtribometer on a hydrogel contact lens. The curve ﬁts using the modiﬁed Winkler foundation model and the Hertzian contact model are shown. The graph to the right shows a small meniscus force during unloading.

fve ¼

Z2p /Zmax 0

0

P/;h R2 sin2 ð/Þ cosðhÞd/ dh

ð13Þ

502

A.C. Rennie et al./Friction coeﬃcient of soft contact lenses

# the Hertzian contact model performed in ﬁgure 3 all of 21=2 1 the terms on the right-hand-side of equation (21) are 3=2 1=2 1=2 fve ¼ pbVR lnð3Þ ln 9 6 Fn ðF n Þ known and can be evaluated for these experimental 2 3 conditions. ð14Þ The reported friction coeﬃcient from the tribometer is a ratio of the sum of all of the friction forces divided 3Fn F n ¼ ð15Þ by the applied normal load as given by equation (23). 2pR3 ks ð23Þ l ¼ ð fve þ fv þ fs =Fn Þ The viscoelastic contribution fve to the friction force Ff is only one component. Two other likely contributors As shown in ﬁgure 3, a meniscus force can be observed to the friction force are an interfacial shear stress be- during unloading in contact experiments. This force was tween the asperities of the glass sphere and the contact found to be on the order of 0.5 mN, and in all sublens fs and the viscous shearing of a ﬂuid ﬁlm within the sequent curve ﬁtting activities the meniscus force was contact fv. This summation of terms is given by equation treated as a constant. Therefore, the actual normal load (16). was assumed to be the sum of the applied normal load and this meniscus force. Ff ¼ fve þ fs þ fv ð16Þ "

2

The frictional force resulting from the shearing of asperities within the contact zone fs is described by equation (17), which assumes an interfacial shear stress ss acts within the apparent area of contact A that is given by equation (18). fs ¼ ss A

ð17Þ

rﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ Fn R0 A ¼ 2p pks

ð18Þ

The viscous shearing force of the ﬂuid ﬁlm within the contact zone is estimated from equation (19), which assumes a Couette ﬂow of the trapped ﬂuid under the contact with a viscosity g0 and an average ﬁlm thickness h. Following traditional elasto-hydrodynamic lubrication theory, it is further assumed that the ﬁlm thickness can be well approximated by expressions for the minimum ﬁlm thickness in soft-elasto-hydrodynamic lubrication given by equation (20) [11]. fv ¼ g0

V A h

h ﬃ hmin ¼ 2:8R00:77 ðg0 VÞ0:65 E 0

ð19Þ 0:44

Fn0:21

ð20Þ

Combining equations (19) and (20) give an expression for the viscous shearing contribution to the friction force fv, which is given by equation (21). In this expression the eﬀective elastic modulus E¢ is given by equation (22). 00:27 0:5 ks fv ¼ 1:266ðg0 VÞ0:35 E00:44 F0:71 n R

E0 ¼ 2

E 1 m2

ð21Þ ð22Þ

The viscosity for the packing solution used in this study is reported to be g0=0.002 Pa s, and the geometric variables are known, as are the sliding speed and normal load. Finally, using the results from the curve ﬁtting of

4. Results and discussion A typical position dependent friction plot is shown in ﬁgure 4(a). The ﬁrst cycle data stands apart from the others because the testing begins with no tangential strain in the ﬂexure. The linear portion of the graph that plots friction coeﬃcient versus lens position is related to the ratio of the tangential and normal stiﬀnesses of the cantilever and is a result of the sphere moving without slip along with the lens during direction reversals. The curvatures in plot of friction coeﬃcient cannot be explained by positional changes in the normal load, which is shown in ﬁgure 4(b), or curvature of the lens. The increases in friction coeﬃcient with time are believed to be a result of the lens drying out during testing as opposed to irreversible damage to the contact lens. Nearly identical initial values of friction coeﬃcient on the same hydrogel lens were obtained in diﬀerent tests where the lens was allowed to rehydrate in the packaging solution between tests. To further test this hypothesis the drying rate was increase by forcing dry argon across the interface; the friction coeﬃcient increased rapidly during the intervals of argon ﬂow. Figure 5(a) plots the average values of friction force, excluding the reversal zones, from cycles 2–10 for 14 diﬀerent experimental tests. Each data point is from a single contact lens sample and a new contact lens was used for each test. The loads varied from 10 to 50 mN and the sliding speeds varied from 63 to 6280 lm/s. Based on ﬁgure 3, estimates of the contact pressure range for this study is believed to be from 54 to 120 kPa. These pressures are an order of magnitude higher than the estimates of contact pressure experienced in the eye and the speeds are an order of magnitude lower. This range of contact pressure and load are near the limits of operation for the reciprocating microtribometer used in this study, and decreasing contact pressure and increasing reciprocating speed are left for future work. The general trend in this data is that friction force

A.C. Rennie et al./Friction coefﬁcient of soft contact lenses

503

Figure 4. (a) Reported friction coeﬃcient versus cycle number and contact lens position. The arrows denote sliding direction of the contact lens. (b) Measured normal load for the same tests. The experimental conditions were V = 100 lm/s and the normal load was 9 mN. The maximum variation in normal load is less than 0.5%.

Figure 5. (a) Friction force for 14 tests varying normal load and sliding speed plotted versus normal load. (b) Reported friction coeﬃcient versus applied normal load on a log–log plot with power-law curve ﬁts.

Figure 6. Comparison of the experimental data plotted in ﬁgure 5 to the curve ﬁt model of equation (16), where the two free parameters are the viscous dissipation coeﬃcient b, and interfacial shear stress ss. The values of these curve-ﬁt parameters and the contributions of each term are shown in the graphs to the right.

504

A.C. Rennie et al./Friction coeﬃcient of soft contact lenses

Figure 7. (a) Reported friction coeﬃcient versus sample position for tests run on a ﬂat hydrogel surface under 9 mN of applied normal load. The friction force data is plotted versus sliding speed in (b). The data collected during reversals is denoted by white circles, and 7 complete cycles are plotted.

increases with increasing normal load and increasing sliding speed. In ﬁgure 5(b) the reported friction coeﬃcient is plotted versus the applied normal load on a log– log plot. The power law dependence with normal load to the )0.4 to )0.5 power is expected based on equation (23), which suggest that the dependence should be between )0.3 and )0.5. In ﬁgure 6 the experimental data is curve ﬁt to equation (23) with two free parameters: (1) the viscous dissipation coeﬃcient b, and (2) the interfacial shear stress ss. The ﬁts are not excellent although they do capture the trends in the experimental data. The contribution of each of the three components of the friction force (viscoelastic, hydrodynamic, and surface shear stress) are shown to the right of the plot. The viscoelastic deformation and the surface shear stress make up the majority of the friction force, with the hydrodynamic contribution representing about 10% of the total. It is of note that the calculated ﬁlm thicknesses using equation (20) were between 1 and 30 nm over the entire experimental range, which suggests that the contact is in boundary lubrication not full elastohydrodynamic lubrication. The curvature in positional friction coeﬃcient data was puzzling until tests were run on specially prepared ﬂat hydrogels of the same Etaﬁlcon-A material. Figure 7(a) shows all the data from a test on one of these samples (7 cycles were run), and the maximum in friction coeﬃcient with central track position is again visible. Following the hypothesis of a velocity dependent friction coeﬃcient, this same data is plotted versus reciprocating speed and the linear slope of friction force with reciprocating speed for the non-reversal zone data is apparent (ﬁgure 7(b)). Additionally, the slopes do not go through 0, which is another indication that the contact is not in full hydrodynamic lubrication.

5. Conclusion Friction tests were run on commercially available contact lenses under a range of contact pressures and speeds. The friction forces were found to be comprised of 3 components: viscoelastic dissipation, interfacial shear, and viscous shearing. A model to account for each of these contributions was developed and ﬁt to the experimental data. This curve ﬁtting exercise suggested that the majority of the frictional forces were due to the viscoelastic dissipation of the contact lens material and interfacial shear within the contact. Acknowledgments The authors gratefully acknowledge the support for Miss Rennie from the University of Florida Undergraduate Scholars Program and the support for Mrs. Dickrell from the University of Florida Minority Fellowship. Additionally ﬁnancial support from Vistakon and helpful conversations with Dr. Jim Jen and Mr. Rangi Raga are greatly appreciated. References [1] [2] [3] [4] [5] [6] [7] [8] [9] [10] [11] [12]

D.K. Martin and B.A. Holden, Phys. Med. Biol. 31 (1986) 635. C.W. McCutchen, Wear 5 (1962) 1. J.A. Nairn and T. Jiangizaire (1995), ANTEC ’95 3384. M.E. Freeman, M.J. Furey, B.J. Love and J.M. Hampton, Wear 241 (2000) 129. G. Hung, F. Hsu and L. Stark, Am. J. Optometr. Physiol. Optics 54 (1977) 678. M.D. Pascovici and T. Cicone, Tribol. Int. 36 (2003) 791. H.W. Liu and B. Bhushan, J. Vacuum Sci. Technol. A 21 (2003) 1528. M.D.P. Willcox, N. Harmis, B.A. Cowell, T. Williams and B.A. Holden, Biomaterials 22 (2001) 3235. P. Podra and S. Andersson, Wear 207 (1997) 79. J. Halling, T.L. Whomes, P.B. Davies and R.D. Arnell, Tribology: Principles and Design Applications (Springer Verlag, 1993). B.J. Hamrock and D. Dowson, J. Lubricat. Technol.—Trans. Asme 100 (1978) 236. S.H. Kim, A. Opdahl, C. Marmo and G.A. Somorjai, Biomaterials 23 (2002) 1657.

Tribology Letters, Vol. 18, No. 4, April 2005 ( 2005) DOI: 10.1007/s11249-005-3610-0

Friction coefﬁcient of soft contact lenses: measurements and modeling A.C. Rennie, P.L. Dickrell and W.G. Sawyer* Department of Mechanical and Aerospace Engineering, University of Florida, Gainesville, FL 32611, USA

Received 12 October 2004; accepted 16 January 2005

Tribological conditions for contact lenses have very low contact pressures in the range 3–5 kPa and sliding speeds around 12 cm/s. Using a microtribometer a series of experiments was run on commercially available contact lenses made from Etaﬁlcon-A. These tests were run using 10–50 mN of normal load at speeds from 63 to 6280 lm/s using a 1-mm radius glass sphere as a pin. The resulting contact pressures are believed to be nearly an order of magnitude larger than the targeted 3–5 kPa. It is hypothesized that the viscoelastic nature of the hydrogel, viscous shearing of the packaging solution, and interfacial shear between the glass sphere and the contact lens all contribute to the friction forces. A model that includes all three of these contributors is developed and compared to the experimental data. The experimental friction coeﬃcients vary from l = 0.025 to 0.075. The calculated ﬂuid ﬁlm thicknesses were between 1 and 30 nm. The average surface roughness of the lens and the glass sphere are Ra=15 nm and Ra=8 nm, respectively, suggesting that the contact is not in full elastohydrodynamic lubrication. Finally, the largest contributors to the friction force in these experiments were found to be viscous dissipation within the hydrogel and interfacial shear within the contact zone. KEY WORDS: contact lens, hydrogel friction, microtribology, microtribometer

1. Introduction Hydrogels are polymer matrices that contain 30–70% water [1] and are the primary material for soft contact lenses. Although soft materials are well suited for the eye, a signiﬁcant fraction of people are unable to wear contact lenses because of extensive eye irritation. There is an existing clinical hypothesis that ocular comfort is related to friction. The mechanical properties of hydrogels are extremely sensitive to water content and humidity, and contact pressure is known to cause redistribution and/or reduction of the water content of hydrogel materials [2]. Therefore, tribological testing of hydrogels must be done under low contact pressure conditions. Nairn and Jiang [3] reported the friction coeﬃcients of polyhydroxy ethyl methacrylate (p-HEMA) based lenses to be in the range of l = 0.060–0.115 using a custom-built pin-on-disk tribometer. The contact pressure in their study was 3.5 kPa. Freeman et al. [4] reported the friction coeﬃcient of ﬂat disks of p-HEMA hydrogels to be in the range of l = 0.02–1.7 over a wide range of applied load, lubrication, hydrogel crosslink density, and degree of hydrogel hydration again using a special purpose tribometer. This study aims to identify the various contributions to friction force in a microtribological contact with a saturated hydrogel. The in vitro conditions are selected *To whom correspondence should be addressed. E-mail: [email protected]ﬂ.edu

to come as close as possible to the pressures and speeds experienced in vivo using existing microtribometry. Blinking is assumed to be the primary force and motion contribution for contact lens tribology. Estimates of the contact pressure created by the eyelid during blinking range from 3.5 to 4.0 kPa and blinking speed average around 12 cm/s [3,5,6]. This combination of low contact pressure and moderate sliding speed are challenging. In this study a reciprocating microtribometer is used to explore the contact pressure and speed dependence of friction coeﬃcient measurements of contact lenses.

2. Experimental setup Tribology experiments were run on a reciprocating microtribometer that uses dual glass ﬂexures to apply mN-range normal loads and react mN-range frictional forces [7]. The tribometer is mounted on an active vibration isolation granite table inside a softwall cleanroom. The apparatus is shown in ﬁgure 1. For these experiments commercially available soft contact lenses made from Etaﬁlcon-A [8] were mounted onto plastic base curves that match the internal radius of curvature of the lenses. The pin sample is a borosilicate crown glass sphere of radius 1mm, and the base curves and contact lenses have a radius of curvature of approximately 7.1 mm. Material properties and surface characterization of the samples are given in table 1. All tests were run using the same experimental procedure: (1) a clean and dry base curve is positioned on 1023-8883/05/0400–0499/0 2005 Springer Science+Business Media, Inc.

500

A.C. Rennie et al./Friction coeﬃcient of soft contact lenses Table 2. Experimental conditions. Applied normal load Reciprocating amplitude Reciprocating frequency Sliding speed Relative humidity Sampling rate

Figure 1. Photograph of the micro-tribometer setup showing: (1) glass ﬂexure to react normal load and friction forces, (2) optical sensor for vertical deﬂections, (3) mirrors, (4) optical sensor for horizontal deﬂections, (5) borosilicate crown glass pin with a 7 mm radius of curvature (a) 1-mm radius sphere was used in this study), (6) EtaﬁlconA contact lens, (7) reciprocating stage, (8) LVDT for stage position measurements, and (9) plastic base curve used to hold the contact lens. Table 1. Material properties of the glass sphere and the Etaﬁlcon-A contact lenses. Glass sphere Average roughness Radius of curvature Elastic modulus Poisson ratio Thickness a

Ra R E m c

a

8 nm 1 mmb 60 GPab 0.30

Contact lens 15 nm[12] 7.1 mmb 255 kPab 0.45b 100 lmb

Collected using a scanning white-light interferometer. Manufacturer reported values.

b

the microtribometer reciprocating stage, (2) a clean and dry glass sphere is mounted to the glass cantilever, (3) a new contact lens package is opened, (4) the lens is removed from the package by hand (only the back side

Fn

V

3–20 mN 0.60 mm 0.07–6.66 Hz 63–6280 lm/s 46–51% 100 Hz

of the lens is handled), (5) the lens is transferred onto the base curve, (6) ﬁnal positioning of the lens on the base curve is done with clean stainless steel tweezers, (7) the lens and base curve assembly is positioned under the borosilicate pin near the apex of the curve, (8) a normal load is applied, and (9) the test is initiated and run for a prescribed number of cycles (based on sliding speed). Steps 3–8 are completed in less than 1 min or the test is abandoned. The experimental conditions used in this study are given in table 2.

3. Modeling The modeling of the experiments done on these contact lenses begins by assuming that the lens can be reasonably modeled with a modiﬁed Winkler surface [9]. The modiﬁcation is the inclusion of a viscous damper into the traditional bed-of-springs elements. This is given by equation (1) where P (Pa) is the contact pressure, E (Pa) is the elastic modulus, m is Poisson’s ratio, c (mm) is the thickness, d (mm) is the normal deformation, b ((Pa s)/mm) is the viscous coeﬃcient, and d_ (mm/s) is the rate of normal deformation. A contact schematic is shown in ﬁgure 2. P¼

E d þ bd_ ¼ ks d þ bd_ ð1 v2 Þc

ð1Þ

The normal load Fn for quasi-static indentation of two spheres can be found by integrating equation (1) over

–

–

–

Figure 2. A contact schematic and nomenclature showing the modiﬁed Winkler foundation material model. The meniscus, lens thickness, ﬂuid ﬁlm thickness, surface roughness, and deformation are all exaggerated.

501

A.C. Rennie et al./Friction coefﬁcient of soft contact lenses

the circular contact of diameter 2b in polar coordinates, where r is the radial coordinate going from 0 to b, and h is the angular coordinate with h=0 lying along the direction of travel. Fn ¼

Z2p Zb 0

P rdr dh ¼ ks

0

Z2p Zb 0

d rdr dh ﬃ ks

pb4 4R0

ð2Þ

0

In equation (2), R¢ is the composite radius of curvature as given by equation (3), where R1 and R2 are the radii of curvature of the two spheres. The approach of centers d for this contact is given by equation (4). The relationship between d and Fn requires solving equation (2) for the contact radius and inserting this result into equation (4). 1 1 1 ¼ þ 0 R R1 R2 d ¼ R1 þ R2

qﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ qﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ R21 b2 R22 b2

ð3Þ

ð4Þ

For the Hertzian contact problem the approach of centers is given by equation (5) [10], where the eﬀective elastic modulus E¢ is given by equation (6) (the borosilicate glass sphere is assumed to be rigid with respect to the contact lens material). 1=3 1 9 F2n d¼ ð5Þ 2 2 E02 R0 E0 ﬃ

E 1 m2

A plot of the normal load versus ﬁlm penetration is shown in ﬁgure 3, and curve ﬁts of equations (4) and (5) are shown on the plot. From these curve ﬁts an elastic modulus E for the foundation model (equation (1)) and a Hertzian contact model (equation (5)) are selected (for both models m=0.45 is used in the curve ﬁtting). It is

noteworthy that the elastic modulus for the foundation model was found to be 260 kPa and the manufacturer reported modulus is 255 kPa. In ﬁgure 2, a schematic for a sphere sliding across the modiﬁed elastic foundation with viscous damping is shown. The deformation d under the sphere of radius R is given in polar coordinates by equation (7). The rate of change of the deformation under the sphere is given by equation (8), where V is the sliding speed. pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ d ¼ d R þ R2 r2 ð7Þ r cosðhÞV d_ ¼ pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ R2 r2

ð8Þ

Combining equations (4), (7) and (8) gives a compact expression for the pressure distribution under a moving sphere, which is given by equation (9). Because of the (h) term in the viscous damping portion of the foundation model, the contribution of this additional term to the integrated pressure distribution is zero (i.e. the contact area remains constant for any sliding speed and thus equation (2) holds for all sliding speeds that do not create negative pressures under the contact). hpﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃi r cosðhÞV 2 2 2 2 Pr;h ¼ R r R b ks þ pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ b ð9Þ R2 r2 Using the substitution r ¼ R sinð/Þ the pressure distribution acting normal to the glass sphere is given by equation (10). The contact zone is over the range of angular coordinate / from / ¼ 0 to /max, which is given in equation (11). P/;h ¼ ½Rðcosð/Þ cosð/max ÞÞks þ ½cosðhÞ tanð/ÞVb ð10Þ /max ¼ sin1

b R

ð11Þ

The diﬀerential friction force, dfve, is the projection of the normal pressure on the sphere opposing the direction of motion multiplied by the diﬀerential area, which is given in equation (12). dfve ¼ P/;h sinð/Þ cosðhÞ dA

ð12Þ

The asymmetric pressure distribution (equation (10)) of the viscoelastic foundation model results in a net friction force fve for this contact geometry. The integral for the viscoelastic contribution to friction force is given by equation (13), and the solution to this integral is given by equation (14), where the dimensionless normal load Fn* is given by equation (15). Figure 3. Experimental data collected by performing an indentation test with the microtribometer on a hydrogel contact lens. The curve ﬁts using the modiﬁed Winkler foundation model and the Hertzian contact model are shown. The graph to the right shows a small meniscus force during unloading.

fve ¼

Z2p /Zmax 0

0

P/;h R2 sin2 ð/Þ cosðhÞd/ dh

ð13Þ

502

A.C. Rennie et al./Friction coeﬃcient of soft contact lenses

# the Hertzian contact model performed in ﬁgure 3 all of 21=2 1 the terms on the right-hand-side of equation (21) are 3=2 1=2 1=2 fve ¼ pbVR lnð3Þ ln 9 6 Fn ðF n Þ known and can be evaluated for these experimental 2 3 conditions. ð14Þ The reported friction coeﬃcient from the tribometer is a ratio of the sum of all of the friction forces divided 3Fn F n ¼ ð15Þ by the applied normal load as given by equation (23). 2pR3 ks ð23Þ l ¼ ð fve þ fv þ fs =Fn Þ The viscoelastic contribution fve to the friction force Ff is only one component. Two other likely contributors As shown in ﬁgure 3, a meniscus force can be observed to the friction force are an interfacial shear stress be- during unloading in contact experiments. This force was tween the asperities of the glass sphere and the contact found to be on the order of 0.5 mN, and in all sublens fs and the viscous shearing of a ﬂuid ﬁlm within the sequent curve ﬁtting activities the meniscus force was contact fv. This summation of terms is given by equation treated as a constant. Therefore, the actual normal load (16). was assumed to be the sum of the applied normal load and this meniscus force. Ff ¼ fve þ fs þ fv ð16Þ "

2

The frictional force resulting from the shearing of asperities within the contact zone fs is described by equation (17), which assumes an interfacial shear stress ss acts within the apparent area of contact A that is given by equation (18). fs ¼ ss A

ð17Þ

rﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ Fn R0 A ¼ 2p pks

ð18Þ

The viscous shearing force of the ﬂuid ﬁlm within the contact zone is estimated from equation (19), which assumes a Couette ﬂow of the trapped ﬂuid under the contact with a viscosity g0 and an average ﬁlm thickness h. Following traditional elasto-hydrodynamic lubrication theory, it is further assumed that the ﬁlm thickness can be well approximated by expressions for the minimum ﬁlm thickness in soft-elasto-hydrodynamic lubrication given by equation (20) [11]. fv ¼ g0

V A h

h ﬃ hmin ¼ 2:8R00:77 ðg0 VÞ0:65 E 0

ð19Þ 0:44

Fn0:21

ð20Þ

Combining equations (19) and (20) give an expression for the viscous shearing contribution to the friction force fv, which is given by equation (21). In this expression the eﬀective elastic modulus E¢ is given by equation (22). 00:27 0:5 ks fv ¼ 1:266ðg0 VÞ0:35 E00:44 F0:71 n R

E0 ¼ 2

E 1 m2

ð21Þ ð22Þ

The viscosity for the packing solution used in this study is reported to be g0=0.002 Pa s, and the geometric variables are known, as are the sliding speed and normal load. Finally, using the results from the curve ﬁtting of

4. Results and discussion A typical position dependent friction plot is shown in ﬁgure 4(a). The ﬁrst cycle data stands apart from the others because the testing begins with no tangential strain in the ﬂexure. The linear portion of the graph that plots friction coeﬃcient versus lens position is related to the ratio of the tangential and normal stiﬀnesses of the cantilever and is a result of the sphere moving without slip along with the lens during direction reversals. The curvatures in plot of friction coeﬃcient cannot be explained by positional changes in the normal load, which is shown in ﬁgure 4(b), or curvature of the lens. The increases in friction coeﬃcient with time are believed to be a result of the lens drying out during testing as opposed to irreversible damage to the contact lens. Nearly identical initial values of friction coeﬃcient on the same hydrogel lens were obtained in diﬀerent tests where the lens was allowed to rehydrate in the packaging solution between tests. To further test this hypothesis the drying rate was increase by forcing dry argon across the interface; the friction coeﬃcient increased rapidly during the intervals of argon ﬂow. Figure 5(a) plots the average values of friction force, excluding the reversal zones, from cycles 2–10 for 14 diﬀerent experimental tests. Each data point is from a single contact lens sample and a new contact lens was used for each test. The loads varied from 10 to 50 mN and the sliding speeds varied from 63 to 6280 lm/s. Based on ﬁgure 3, estimates of the contact pressure range for this study is believed to be from 54 to 120 kPa. These pressures are an order of magnitude higher than the estimates of contact pressure experienced in the eye and the speeds are an order of magnitude lower. This range of contact pressure and load are near the limits of operation for the reciprocating microtribometer used in this study, and decreasing contact pressure and increasing reciprocating speed are left for future work. The general trend in this data is that friction force

A.C. Rennie et al./Friction coefﬁcient of soft contact lenses

503

Figure 4. (a) Reported friction coeﬃcient versus cycle number and contact lens position. The arrows denote sliding direction of the contact lens. (b) Measured normal load for the same tests. The experimental conditions were V = 100 lm/s and the normal load was 9 mN. The maximum variation in normal load is less than 0.5%.

Figure 5. (a) Friction force for 14 tests varying normal load and sliding speed plotted versus normal load. (b) Reported friction coeﬃcient versus applied normal load on a log–log plot with power-law curve ﬁts.

Figure 6. Comparison of the experimental data plotted in ﬁgure 5 to the curve ﬁt model of equation (16), where the two free parameters are the viscous dissipation coeﬃcient b, and interfacial shear stress ss. The values of these curve-ﬁt parameters and the contributions of each term are shown in the graphs to the right.

504

A.C. Rennie et al./Friction coeﬃcient of soft contact lenses

Figure 7. (a) Reported friction coeﬃcient versus sample position for tests run on a ﬂat hydrogel surface under 9 mN of applied normal load. The friction force data is plotted versus sliding speed in (b). The data collected during reversals is denoted by white circles, and 7 complete cycles are plotted.

increases with increasing normal load and increasing sliding speed. In ﬁgure 5(b) the reported friction coeﬃcient is plotted versus the applied normal load on a log– log plot. The power law dependence with normal load to the )0.4 to )0.5 power is expected based on equation (23), which suggest that the dependence should be between )0.3 and )0.5. In ﬁgure 6 the experimental data is curve ﬁt to equation (23) with two free parameters: (1) the viscous dissipation coeﬃcient b, and (2) the interfacial shear stress ss. The ﬁts are not excellent although they do capture the trends in the experimental data. The contribution of each of the three components of the friction force (viscoelastic, hydrodynamic, and surface shear stress) are shown to the right of the plot. The viscoelastic deformation and the surface shear stress make up the majority of the friction force, with the hydrodynamic contribution representing about 10% of the total. It is of note that the calculated ﬁlm thicknesses using equation (20) were between 1 and 30 nm over the entire experimental range, which suggests that the contact is in boundary lubrication not full elastohydrodynamic lubrication. The curvature in positional friction coeﬃcient data was puzzling until tests were run on specially prepared ﬂat hydrogels of the same Etaﬁlcon-A material. Figure 7(a) shows all the data from a test on one of these samples (7 cycles were run), and the maximum in friction coeﬃcient with central track position is again visible. Following the hypothesis of a velocity dependent friction coeﬃcient, this same data is plotted versus reciprocating speed and the linear slope of friction force with reciprocating speed for the non-reversal zone data is apparent (ﬁgure 7(b)). Additionally, the slopes do not go through 0, which is another indication that the contact is not in full hydrodynamic lubrication.

5. Conclusion Friction tests were run on commercially available contact lenses under a range of contact pressures and speeds. The friction forces were found to be comprised of 3 components: viscoelastic dissipation, interfacial shear, and viscous shearing. A model to account for each of these contributions was developed and ﬁt to the experimental data. This curve ﬁtting exercise suggested that the majority of the frictional forces were due to the viscoelastic dissipation of the contact lens material and interfacial shear within the contact. Acknowledgments The authors gratefully acknowledge the support for Miss Rennie from the University of Florida Undergraduate Scholars Program and the support for Mrs. Dickrell from the University of Florida Minority Fellowship. Additionally ﬁnancial support from Vistakon and helpful conversations with Dr. Jim Jen and Mr. Rangi Raga are greatly appreciated. References [1] [2] [3] [4] [5] [6] [7] [8] [9] [10] [11] [12]

D.K. Martin and B.A. Holden, Phys. Med. Biol. 31 (1986) 635. C.W. McCutchen, Wear 5 (1962) 1. J.A. Nairn and T. Jiangizaire (1995), ANTEC ’95 3384. M.E. Freeman, M.J. Furey, B.J. Love and J.M. Hampton, Wear 241 (2000) 129. G. Hung, F. Hsu and L. Stark, Am. J. Optometr. Physiol. Optics 54 (1977) 678. M.D. Pascovici and T. Cicone, Tribol. Int. 36 (2003) 791. H.W. Liu and B. Bhushan, J. Vacuum Sci. Technol. A 21 (2003) 1528. M.D.P. Willcox, N. Harmis, B.A. Cowell, T. Williams and B.A. Holden, Biomaterials 22 (2001) 3235. P. Podra and S. Andersson, Wear 207 (1997) 79. J. Halling, T.L. Whomes, P.B. Davies and R.D. Arnell, Tribology: Principles and Design Applications (Springer Verlag, 1993). B.J. Hamrock and D. Dowson, J. Lubricat. Technol.—Trans. Asme 100 (1978) 236. S.H. Kim, A. Opdahl, C. Marmo and G.A. Somorjai, Biomaterials 23 (2002) 1657.